AlN Thin Film Electroacoustic Devices


 Oswin Sparks
 1 years ago
 Views:
Transcription
1 Comprehensive Summaries of Uppsala Dissertations from the Faculty of Science and Technology 817 AlN Thin Film Electroacoustic Devices BY GONZALO FUENTES IRIARTE ACTA UNIVERSITATIS UPSALIENSIS UPPSALA 2003
2 AlN Thin Film Electroacoustic Devices 1 A Sabina Iriarte Ilintxeta, mi madre.
3 G.F.Iriarte 2 Dissertation for the Degree of Doctor of Philosophy in Solid State Electronics presented at Uppsala University in 2003 ABSTRACT Iriarte, G.F AlN Thin Film Electroacoustic Devices. Acta Universitatis Upsaliensis. Comprehensive Summaries of Uppsala Dissertations from the Faculty of Science and Technology pp. Uppsala. ISBN Recently, the enormous growth in personal communications systems (PCS), satellite communication and various other forms of wireless data communication has made analogue frequency control a key issue as the operation frequency increases to the low/medium GHz range. Surface acoustic wave (SAW) and bulk acoustic wave (BAW) electroacoustic devices are widely used today in a variety of applications both in consumer electronics as well as in specialized scientific and military equipment where frequency control is required. Conventional piezoelectric materials such as quartz, LiNbO3 and LiTaO3 suffer from a variety of limitations and in particular medium to low SAW/BAW velocity as well as being incompatible with the IC technology. Thin piezoelectric films offer the great flexibility of choosing at will the substrate/film combination, thus making use of the electroacoustic properties of nonpiezoelectric substrates, which widens greatly the choice of fabrication materials and opens the way for integration of the traditionally incompatible electroacoustic and IC technologies. This thesis focuses on the synthesis and characterization of novel thin film materials for electroacoustic applications. A prime choice of material is thin piezoelectric AlN films which have been grown using both RF and pulseddc reactive sputter deposition on a variety of substrate materials. A unique synthesis process has been developed allowing the deposition of high quality AlN films at room temperature, which increases greatly the process versatility. The films are fully caxis oriented with a 1.6 FWHM value of the rocking curve of the AlN(002) peak. Complete process flows for the fabrication of both SAW and BAW devices have been developed. Electroacoustic characterization of 2 GHz BAW resonators yielded an electromechanical coupling coefficient (kt²) of 6.5%, Qvalue of 600 and a longitudinal velocity of m/s. AlN thin films based SAW resonators on SiO 2 /Si yielded a SAW velocity of around 5000 m/s and a piezoelectric coupling coefficient (K²) of around 0.3%. Finally, AlN on polycrystalline diamond 1 GHz SAW resonators exhibited an extremely high SAW velocity of m/s, a piezoelectric coupling coefficient (K²) of 1% and a Qvalue of 500. G.F.Iriarte, Solid State Electronics, The Ångström Laboratory Uppsala University, Box 534, SE Uppsala, Sweden G.F.Iriarte 2003 ISSN X ISBN Printed in Sweden by Kopieringshuset, Uppsala 2003
4 AlN Thin Film Electroacoustic Devices 3 Publications This thesis is based on the following publications, which in the following will be referred to in the text by their Roman numerals. I. Synthesis of highly oriented piezoelectric AlN films by reactive sputter deposition F. Engelmark, G. Fuentes, I. V. Katardjiev, A. Harsta, U. Smith, and S. Berg J. Vac. Sci. Technol. A, Vol. 18, No. 4, Jul Aug 2000 II. III. IV. Structural and electroacoustic studies of AlN thin films during low temperature radio frequency sputter deposition F. Engelmark, G. F. Iriarte, I. V. Katardjiev, M. Ottosson, P. Muralt, and S. Berg J. Vac. Sci. Technol. A 19(5), Sep Oct 2001 Selective etching of Al/AlN structures for metallization of surface acoustic wave devices F. Engelmark, G. F. Iriarte, and I. V. Katardjiev J. Vac. Sci. Technol. B 20(3), May Jun 2002 Reactive sputter deposition of highly oriented AlN films at room temperature G. F. Iriarte, F. Engelmark, I.V. Katardjiev J. Mater. Res. 17(6), (2002) V. Influence of deposition parameters on the stress of magnetron sputterdeposited AlN thin films on Si (100) substrates. G. F. Iriarte, F. Engelmark, M. Ottosson, I.V. Katardjiev. J. Mater. Res. 18(2), (2003) VI. Electrical Characterization of AlN MIS and MIMstructures F. Engelmark, J. Westlinder, G. F. Iriarte, I. V. Katardjiev, J. Olsson Submitted to IEEE Transactions on Electron Devices (2002) VII. Synthesis of CAxis Oriented AlN Thin Films on Metal Layers: Al, Mo, Ti, TiN and Ni. G. F. Iriarte, J. Bjurström, J. Westlinder, F. Engelmark, I.V. Katardjiev. Submitted to IEEE Transactions on Ultrasonics, Ferroelectrics and Frequency Control (2002) VIII. SAW propagation characteristics of AlN thin films grown on polycrystalline diamond substrates at room temperature. G.F.Iriarte Submitted to Journal of Applied Physics 3 February Accepted 3 March IX. SAW COMparameter extraction in AlN/diamond layered structures. G. F. Iriarte, F. Engelmark, I.V. Katardjiev, V.Plessky, V.Yantchev Submitted to IEEE Transactions on Ultrasonics, Ferroelectrics and Frequency Control (2003)
5 G.F.Iriarte 4
6 AlN Thin Film Electroacoustic Devices 5 Contents 1. Introduction Theoretical aspects Acoustic Wave Excitation Layered structures for SAW applications Theoretical background Dispersion curves Modelling techniques for SAW Devices Modelling techniques for BAW Devices Process Technology Low Density Plasmas Particle Energies in low density plasmas Potential distribution in a plasma DC Plasma discharges Magnetron sputtering RF Plasma discharges Pulsed DC Plasma discharges Synthesis of AlN Thin Films Nucleation and growth of thin films Reactive sputtering Lithography and Etching Analytical techniques Xray Diffraction Atomic Force Microscopy (AFM) Scanning Electron Microscopy (SEM) Transmission Electron Microscopy (TEM) Electron Spectroscopy for Chemical Analysis (ESCA) Summary of Papers...40 Acknowledgements...60 References...61
7 G.F.Iriarte 6
8 AlN Thin Film Electroacoustic Devices 7 1. Introduction Acoustic wave devices based on piezoelectric materials have been in commercial use for over 60 years[1]. They are used in a wide variety of applications such as delay lines, oscillators, resonators, sensors, actuators, acoustic microscopy as well as in specialized military equipment but by far the largest market is the telecommunication industry, primarily for wireless communication in mobile cell phones and base stations. This industry consumes annually approximately three billion acoustic wave filters for frequency control. The filters are typically based on surface acoustic wave (SAW) and bulk acoustic wave (BAW) resonator technology. Commonly used piezoelectric materials in SAW devices are single crystalline substrates of quartz (SiO 2 ), lithium tantalate (LiTaO 3 ) and lithium niobate (LiNbO 3 ). Other wellestablished resonator technologies are standard onchip LC, transmission lines and ceramic resonators. Recently, the enormous growth in personal communications systems (PCS), satellite communication and various other forms of wireless data communication has made analogue frequency control a key issue as the operation frequency increases to the low/medium GHz range. Also, the technological drive to minimise and improve the capacity of such systems has shown the need for the development of high performance, miniature, onchip filters operating in the low and medium GHz frequency range. At the frequency of interests, other resonator technologies such as LC, ceramic resonators and transmission line resonators become too large for wireless applications[2]. One of the biggest disadvantages of the electroacoustic technology in the microwave region is that it makes use of bulk single crystalline piezoelectric materials, the choice of which is rather limited and which by definition are incompatible with the IC technology. In addition, the properties of these materials determine uniquely the acoustic velocity, which in turn together with the device dimensions define the operating frequency. Thus, the only way to increase the latter is to decrease the device dimensions which comes at an enormous increase in the fabrication costs, both for BAW and SAW devices particularly in the microwave region. In recent years thin piezoelectric films have been developed to extend electromechanical SAW and BAW devices to much higher frequencies[3, 4]. The standard electroacoustic technology, however, continues and will continue to dominate the market for devices operating, say, under 2 GHz. For higher frequencies up to 20 GHz, on the other hand Thin Film Bulk Acoustic Resonators (TFBAR or FBAR) is considered to be the most promising approach today because they are characterised by small dimensions, low losses, high power handling capabilities and not the least low fabrication cost. In addition, this approach allows the great flexibility of choosing at will the substrate/film combination, thus making use of the electroacoustic properties of the nonpiezoelectric substrate and widening greatly the choice of fabrication materials. Thus, a whole new variety of thin piezoelectric films can be grown on arbitrary substrates. This approach also makes use of the highly developed thin film technology, where thin films of extremely high uniformity and controlled properties can be grown on large area
9 G.F.Iriarte 8 substrates. Agilent Technologies[5] is the first company to start mass production of discrete FBAR devices in Q It should be strongly pointed out, however, that by far the greatest potential of using thin films for the fabrication of FBARs is that it opens the very promising possibility of integrating the traditionally incompatible IC and electroacoustic technologies. This in turn will bring about a number of substantial benefits such as significant decrease in the fabrication cost of the final device, easier and simpler device design as well as increased sensitivity, reduced losses, power consumption, device size, materials use, electromagnetic contamination, etc. Another very significant benefit of this integration would be the mass fabrication of highly sensitive, low cost integrated chemical and biological sensors and electronic tags. Environmental control is becoming of great importance for today's society both for the manufacturing industry and public activities. The increasing threat of chemical and biological sabotage along with that of hazardous industrial incidents necessitate large scale monitoring of the environment which can only be done by mass produced low cost sensors. Thus, the research in this field is centred around the development of novel functional materials (piezoelectric, ferroelectric, etc) with superior electroacoustic properties allowing the fabrication of high frequency devices with improved performance and at the same time at low fabrication cost. By the way of example, materials with high piezoelectric coefficients are sought to allow the design of bandpass filters with large bandwidths, say of the order of 10% or more. Further, these materials should exhibit low electroacoustic losses, i.e. should be characterised with a high quality factor as well as high thermal stability in the temperature range of operation. Tunability is also a desirable property for advanced frequency agile and adaptive microwave communications systems. Not the least, the synthesis process should be compliant with the planar technology, while the materials themselves should be compatible with the IC technology. This thesis focuses on the synthesis of highly textured piezoelectric thin AlN films using reactive sputter deposition as well as their electrical and electroacoustic characterisation in view of electroacoustic applications. Among the major goals of the work are the development of a low temperature synthesis process of caxis oriented AlN films, development of a fabrication process flow of thin film based resonators (both SAW and BAW), as well as design, fabrication and characterisation of the latter. The thesis is organised as follows. Chapter 2 presents a summary of the main theoretical models used for the design, description, parameter extraction and characterisation of the thin film resonators. Chapter 3 gives an overview of the fabrication processes used for the fabrication of thin film electroacoustic devices. Finally, Chapter 4 presents a summary of the major results obtained and published in each paper in this thesis in the order of publication.
10 AlN Thin Film Electroacoustic Devices 9 PROPERTIES OF ALUMINIUM NITRIDE (ALN) Aluminium nitride (AlN) thin films are widespread applied because they had some excellent properties such as chemical stability, high thermal conductivity, electrical isolation, a wide band gap (6.2 ev), a thermal expansion coefficient similar to that of GaAs, and a higher acoustic velocity. Therefore, AlN thin films were applied not only to surface passivation of semiconductors and insulators, but also to optical devices in the ultraviolet spectral region, acoustooptic (AO) devices, and surface acoustic wave (SAW) devices. Polycrystalline films exhibit piezoelectric properties and can be used for the transduction of both bulk and surface acoustic waves. If compared to other piezoelectric film, such as the well known ZnO, AlN shows a slightly lower piezoelectric coupling; its Rayleigh wave velocity is close to the maximum in the range of values of most materials, being that of ZnO close to the minimum. The Rayleigh wave phase velocity in ccut AlN (Vph = 5607m/s) is much higher than that of most substrates of practical interest in SAW devices technology. This suggests that AlN and ZnO, rather than alternatives, have to be considered each with its own field of application, with a preference for AlN in high Rayleigh wave velocity substrates and high frequency applications. As to sputter film growth, conditions are more critical for AlN then for ZnO because of the possible presence of strong internal stresses (see Paper V). Results have shown that the growing of high thickness AlN films is rather critical because of its tendency to present microcracking. This tendency is more evident with increasing the thickness of the film and when using silicon substrates, particularly in the (100) orientation. Property Value Band gap 6.2 ev Density 3.3 g/cm3 Theoretical thermal conductivity 320 W/mK Thermal expansion coefficient 4.6E6/ ºC Critical field strength Ec 615 MV/cm Relative dielectric constant εr 8.5 Refractive index n 2.15 Thermal conductivity 2.0 W/cmK Melting point >2000 ºC Lattice constant a Å Lattice constant c Å Table 1 Some data on AlN AlN has a very large volume resistivity. It is a hard material with a bulk hardness similar to quartz, about Kg/mm. Pure AlN is chemically stable to attack by atmospheric gases at temperatures less than about 700 ºC. The combination of these physical and chemical properties has stirred considerable interest in practical application of AlN both in bulk and thinfilm form.
11 G.F.Iriarte Theoretical aspects 2.1. Acoustic Wave Excitation In a piezoelectric medium, the stress (T) and the electric displacement (D) depend linearly on both the strain (S) and the electric field (E), and the equations for D and T become: E (1) T = c S e E (2) ij D i ijkl = e ijk kl S jk kij + ε S ij where εij, eijk and Cijkl are the permittivity, piezoelectric and stiffness tensors respectively. These are called the constitutive equations or equations of state of the system. The superscript E in the stiffness constants denotes that it is measured at constant electric field. Due to the piezoelectric effect, the velocity of propagation of acoustic waves in piezoelectric media is higher than in the nonpiezoelectric case. It is a common practice to modify the stiffness tensor by adding to it elements of the piezoelectric and permittivity tensors as shown in (3), in order to calculate the impact of piezoelectricity in the velocity of propagation of the wave. The stiffness constants in that case are referred to as stiffened. However, a specific crystal may be strongly piezoelectric for a given propagation direction while the effect is completely absent in another direction. Hence, piezoelectricity is always coupled to the direction of propagation or cut of the crystal. For this reason, Euler angles[6] are often used in the literature to render the stiffened stiffness constants into a specific propagation direction[7]. Hence, piezoelectric corrections to the stiffness matrix depend not only on the permittivity [ε] and piezoelectric [e] matrices, which in turn depend on the symmetry class of the material, but also on the direction of propagation of the acoustic wave. For a piezoelectrically stiffened acoustic wave, the phase velocity is determined by (3) k E E 2 ω C e V = = ph 1 + S E k ρ ε C where the subscripts of the tensor components have been dropped for clarity. To determine the piezoelectric correction quantitatively, we use the unstiffened phase velocity (4) V ph = ω k = C ρ E Rewriting the stiffened phase velocity (3) in terms of the unstiffened phase velocity we obtain 1 (5) 2 ( ) 2 V ph = Vph 1+ K where the constant K² is given by j
12 AlN Thin Film Electroacoustic Devices 11 (6) K 2 2 e = S ε C and is called the piezoelectric coupling constant. We also define the electromechanical coupling constant: (7) k 2 t = E D E C = C + e ε 2 S where the subscript refers to the requirement that the electric field is applied across the thickness of the crystal. Clearly, the coupling constants kt and K² are related as 2 (8) 2 K k t = 2 1+ K The reason for the definition of two different types of coupling constants is explained as follows: Basically, plane acoustic waves can be excited in piezoelectric crystals using two different configurations referred to as Lateral Field Excitation (LTE) and Thickness Excitation (TE). The stiffening correction term (in brackets in (3)) involves vectors that correspond to the orientation of the acoustically generated electric field. In TE, these vectors are oriented in the direction of acoustic propagation. In LFE, the vectors are in the direction of the external electric field, which can be oriented arbitrarily in the plane perpendicular to the acoustic propagation. a) Thickness Excitation In Thickness Excitation, an externally generated electric field in the Zdirection in Figure 1 causes the propagation of an acoustic wave in that direction. The implication of the quasistatic approximation (see below) is that the electric field continuously being generated by the strain wave (i.e. acoustically generated) is longitudinal and propagates at the acoustic phase velocity. The internally generated electric field vector is parallel to both the externally applied electric field and the direction of acoustic wave propagation. THICKNESS EXCITATION z x Electrodes y Figure 1 Thickness Excitation (TE) mode. Since the curl of the electric field is zero in the quasistatic case, it implicitly means that the electric displacement vector in the direction of acoustic wave propagation is also zero. This can be shown by considering the characteristic
13 G.F.Iriarte 12 behaviour of a plane acoustic wave travelling in the Zdirection (i.e. the displacement vector and the stress vary only in the Zdirection), thus having a exp [j(ωt  βz)] dependence. Combining of the constitutive equations (1) and (2) and solving for the displacement we get E (9) T ij c S ijkl D = S jk + + S i eijk εij jk ekij ekij Since the only displacement components are in the Zdirection, the strain reduces to (10) u z Sjk = Sz = = jkuz z and Newton s law becomes 2 2 (11) u z Tz ρω ρ = = 2 t z jk Hence, (12) 2 E C S ρω D = + + ( jku ) i e ( jkuz ) ε z  jke e where the subscripts of the tensor components have again been dropped for clarity. Substituting the expression for the piezoelectrically stiffened phase velocity (3) into this equation we find that Dz = 0. The consequence of a vanishing Dz is that in the piezoelectric medium there is a longitudinal electric field without a proportional electric displacement vector. The electrical source does not directly cause a displacement vector (and thus there is no displacement current) in the direction of propagation of the acoustic wave. In other words, it is impossible to extract electric energy from the piezoelectric medium, because there is no displacement current. Energy conversion is accomplished by using resonating structures. Since the electric field is variable, the stiffness components are measured at D constant (zero) electrical displacement D, which explains the use of C in place of E C. In the TE mode, the propagating acoustic wave generates an electric field in the piezoelectric crystal and viceversa. Hence the wave propagation is regarded as stiffened and the coefficient, given by kt, is used to express the coupling in BAW devices using this excitation mode. b) Lateral Field Excitation (LTE) In LFE the electric field is in the plane perpendicular to acoustic propagation. A practical realization of Lateral Field Excitation is shown in Figure 2. The applied (external) electric field is uniform in the Ydirection and the propagation of bulk acoustic waves is in the Zdirection (perpendicular to the electric field). An electric field can excite an acoustic wave normal to its direction because the piezoelectric matrix [e] couples electrical and mechanical fields of different orientations.
14 AlN Thin Film Electroacoustic Devices 13 In Lateral Field Excitation, the internally generated electric field may be accurately assumed to be zero. Hence, the potential Φ is also assumed to be zero. Instead, there is an internally generated electrical displacement vector containing terms that are normal to the direction of acoustic propagation direction and thus parallel to the externally generated electric field. The interaction of the acoustic wave with the source occurs though the electric displacement D, which means that D propagates at the acoustic velocity. The internally generated D vector is parallel to the externally generated electric field vector E. For this reason, in the Lateral Field Excitation mode, the components of stiffness tensor are measured at constant E electric field E, which is denoted as C. LATERAL FIELD EXCITATION z x y Electrodes + _ t d Figure 2 Lateral Field Excitation (LFE) mode. A necessary condition for LFE to exist is that the thickness t of the crystal in Figure 2 must be much smaller that the distance between the electrodes d. Lateral Field Excitation is relevant to static measurements or to dynamic behaviour of piezoelectric crystals that are very small compared to the acoustic wavelength (i.e. t is much smaller than the distance between the electrodes d), but it is not applicable to wave propagation problems where the variables of interest are timedependent as they vary with the acoustic wave. However, due to the analogy in terms of practical realization of devices working in the LFE mode, the coupling constant K² (see Equation (5) above) is used to express the coupling in SAW devices. There is a simple interpretation for K² in terms of the ratio of externally generated electric field energy density to the mechanical energy density[4].
15 G.F.Iriarte Layered structures for SAW applications Theoretical background In a piezoelectric material, surface acoustic waves can be generated and detected electrically by means of metal electrodes at the surface. This principle is used in interdigital transducers (IDTs) and multistrip couplers. If an alternating electric field is applied between the electrodes of an IDT, and as a consequence of the piezoelectric effect, surface acoustic waves will travel away from the transducer in both directions. At the frequency for which the acoustic wavelength is equal to the period of the IDT, the electric field between adjacent electrodes will reach the highest level and all the electrodes will contribute to the generation of the acoustic wave in a cooperative manner. Hence, at that particular frequency, often referred to as the center or the Bragg frequency, electromagnetic waves applied are converted into an acoustic signal with maximal efficiency. Z (x3) Y (x2) X (x1) Figure 3 IDT launching an acoustic wave on a piezoelectric substrate. The coordinate system used is shown to the right. In order to derive the equations governing the propagation of acoustic waves in piezoelectric media (equations of motion), we recall the following assumptions: a) The quasistatic approximation When either of the media through which an acoustic wave propagates is piezoelectric, the problem involves not only the elastic particle displacements but also the electric and magnetic fields, with the result that the applicable equations are combinations of the elastic equations of motion and of Maxwell s equation, intercoupled by the piezoelectric tensors of the media. The intercoupling is usually weak enough for the solutions of the equations to be divided into two classes, those that propagate with acoustic velocities (a few thousand meters per second) and those that propagate with electromagnetic velocities (~ kilometres per second). We will restrict the discussion here to the former class. With this restriction, the magnetic fields can be neglected and the electric fields can be derived from a scalar potential. In other words, since acoustic waves in commonly used materials are about five orders of magnitude slower than electromagnetic
16 AlN Thin Film Electroacoustic Devices 15 waves, the piezoelectrically coupled electric field is assumed to be quasistatic. This assumption is known as the quasistatic approximation. Hence, (13) E i Φ = x For chargefree dielectrics eq.(13) yields: (14) Di = 0 x i i Here, Ei is electric field, Di is electrical displacement, Φ is potential. b) The mechanical equation of motion Newton s second law gives the mechanical equations of motion and for an infinitesimally small volume (i.e. the solid is considered as a continuum medium) it states: 2 3 (15) u T i ij ρ = 2 t x j= 1 i Here, Tij is the stress, and ui denotes particle displacement. In these equations, the summation convention for repeated indices is employed and the tensors are expressed by Einstein's convention. Taking the former assumptions into account, the first derivative of the constitutive relation (equations (1) and (2)) with respect to space, leads us to a set of four coupled wave equations; one for the electric potential Φ and three for the three components of the elastic displacement ui. These are called the wave equations or equations of motion of the system (16) u j uk Φ ρ cijkl ekij = 0 2 t x x x x 2 2 (17) u k Φ eikl ε ik = 0 x x x x i l i l Thus, the equations of motion are derived from the constitutive equations of the media after substituting Newton s second law and the quasistatic approximation. Following Campbell and Jones method[8], the general solution to the wave equation above is assumed to be a linear combination of partial waves given by (18) (19) u i k i ikbx3 ik(x1 vt) j = α j e e, j = 1,2,3 Φ = α e 4 ikbx3 ik(x1 vt) e where the constants α give the relative amplitudes of the displacement components of each partial wave and the decay constants b describe the variation with depth of the amplitude and phase of the partial wave measured on a plane of constant phase i.e. a plane perpendicular to the XZplane in Figure 3. Substituting the partial waves into the wave equation an eighthorder algebraic equation in the decay constants b is obtained. Thus, for each value of the phase velocity Vph, eight k
17 G.F.Iriarte 16 values of b are found in the most general case. Moreover, for each of the eight roots b, there is a fourcomponent eigenvector (α1, α2, α3, α4). When the system is irreductible, it is not always possible to find a solution with the full number of arbitrary functions, but it is possible to construct solutions that contain as many constants as required. In other words, since we have 8 different decay constants b and for each one of this constants b, there is a unique eigenvector (α1, α2, α3, α4), we must find a way to determine one solution (now there are 8 possible solutions). The way to find this unique solution is by combining all the partial waves using weighting factors Cm. This weighting factors can be find out by determining as many boundary conditions as necessary, that means, as many boundary conditions as weighting factors Cm appear in the equation system. The particle displacement and potential in the equations for the partial waves, Equations (18) and (19), are given as eight linear combinations of plane waves. These linear combinations constitute the general solution of the system: 8 m (20) m ikb x 3 ik(x 1 vt) u j = C mα j e e, j=1,2,3. m = 1 (21) Φ = C mα 8 m= 1 m 4 e m ikb x 3 e ik(x 1 vt) So far, the discussion concerns bulk materials. For layered structures, another set of boundary conditions must be satisfied at the interface between adjacent layers. Since the assumption of the semiinfinite substrate is only applicable for the lowest layer, eight unknown constants exist for each layer except for the lowest one. This is so because at the interface between two layers of different materials, the wave is likely to be reflected back towards the surface, hence giving rise to positive values of the decay constants b. For instance, in the case of AlN/diamond structure (studied in Paper VIII and Paper IX), the general solution for the displacement and the potential satisfying (16) and (17) are given as where (22) (23) (24) (25) Dia j u Dia j Φ Dia u AlN j Φ AlN = α = α = α = α Dia j Dia 4 AlN j AlN 4 e e e e ikb Dia x 3 ikbdiax3 ikb AlN x 3 ikbalnx3 e e ik(x 1 vt) ik(x1 vt) e e ik(x 1 vt) ik(x1 vt) α (j = 1,2,3) and α AlN (j = 1,2,3) are constants. Substituting (22) and j (23)into (16) and (17) respectively, the eighthorder equation is obtained for bdia and the eight roots are obtained. Similarly, substituting (24)and (25) for an AlN layer into (16) and (17) respectively, the eighthorder equation is obtained for baln and eight roots are obtained. Therefore, the displacement uj and the potential Φ are expressed as the summation of the linear combinations of eight waves, which are given as
18 AlN Thin Film Electroacoustic Devices 17 8 (m) (26) Dia Dia Dia(m) ikb x 3 ik(x 1 vt) u j = C m α j e Dia e, j=1,2,3. m = 1 (27) Φ = C 8 (m) Dia Dia Dia(m) ikbdiax3 ik(x1 vt) m α4 e e m= 1 8 (m) (28) AlN AlN AlN(m) ikb AlN x 3 ik(x 1 vt) u j = C m α j e e, j=1,2,3. m = 1 (29) Φ = C 8 (m) AlN AlN AlN(m) ikb AlN x 3 ik(x 1 vt) m α4 e e m= 1 Because 90% of the SAW energy concentrates within one wavelength near the surface of the substrate, thick (at least 3 times the acoustic wavelength) piezoelectric substrates are assumed to be semiinfinite substrates. Assuming that the diamond layer is a bulk material (i.e. semiinfinite), four out of the eight b roots are effective to satisfy the condition that the SAW wave does not exist at negative infinity for X3 (see Figure 3). Therefore, (26) and (27) are expressed as follows. 4 (m) (30) Dia Dia Dia(m) ikb x 3 ik(x 1 vt) u j = C m α j e Dia e, j=1,2,3. m= 1 (31) Φ = C 4 (m) Dia Dia Dia(m) ikb Dia x 3 ik(x1 vt) m α4 e e m = 1 For the AlN layer, all eight roots apply. From Equations (28) to (31) it is seen that a total of twelve unknown parameters (four corresponding to the diamond layer and eight corresponding to the AlN layer) appear for the AlN/Diamond structure. Once the equations describing the system have been erected, boundary conditions have to be applied to solve it. These are as follows: The particle displacements and the traction components of stress (T13, T23 and T33) must be continuous across the interface because of the intimate nature of the contact assumed between the two materials. Since the surface is assumed to be mechanically stress free, the three traction components of stress must vanish thereon. The electrical boundary conditions to the problem are provided by the continuity of the potential and of the normal component of electric displacement across both the interface and the free surface. In the case of a layered structure, the conditions of each layer boundary are also required for u, T, D, and the potential for being continuous. For instance, the following conditions apply for the AlN/diamond system at the boundary interface. Dia AlN Dia AlN Dia AlN Dia AlN (32) u = u, T = T, D = D, Φ =Φ i i i 3 i3 i i We are left with twelve boundary conditions for the general problem under consideration. It is convenient to group these boundary conditions into three categories: the mechanical boundary conditions involving transverse displacements and facial stresses, the remaining electrical boundary conditions, and
19 G.F.Iriarte 18 the sagittal plane (XZplane in Figure 3) mechanical boundary conditions. For the twelve unknown parameters, three equations are given by the stress boundary condition at the surface of AlN and one equation is given by the potential at the surface or the electrical displacement boundary condition. Three equations are obtained by the stress boundary condition and three equations by the continuity of each displacement at the interface between diamond and A1N. From the continuity of the normal direction of the electric displacement and the conductivity of the potential at the interface between diamond and A1N, two additional equations are obtained. Hence, the equation system can be solved since it consists of twelve equations with twelve unknown parameters. Substituting this general solution into the wave equation and taking into account the boundary conditions yields the boundarycondition determinant for the general case. Making this determinant equal zero by choosing values of the phase velocity Vph until it is so, we can find out all coefficients b and all coefficients α. After that, the twelve weighting factors Cm can easily be found since we have twelve equations for twelve unknowns Cm and the general expressions for the displacement and for the potential are completely defined. A detailed description of the propagation of acoustic waves in layered structures can be found in Farnell and Adler s work[912], which in its turn has its origin on Campbell and Jones method[8]. Adler s group at McGill Univ., Montreal, Canada, has developed a computer program[1315] based on this approach, which is available on the internet at UFFC website (www.ieeeuffc.com) Dispersion curves The method described is very useful in the design process of SAW devices since it permits to calculate the propagation velocity of the acoustic wave in a given direction in the material. Moreover, since the values of the phase velocity depend on the decay constants b, it is clear that the velocity of the acoustic wave will depend on the thickness of the layer of material though which it propagates, in other words, it will be dispersive. The determination of the exact velocity of propagation of the acoustic wave is essential in the design process since it determines the center frequency of the device. Acoustic losses can be accounted for in the model by including the viscous damping of the medium which in practice is implemented by introducing complex stiffness constants[7]. Another very important result is the possibility to calculate the piezoelectric coupling coefficient, a parameter of primary importance for the design of electroacoustic devices. In a layered surface acoustic wave device, where an array of electrode stripes is used to excite the acoustic wave, the location of the electrodes with respect to the layers can drastically affect the coupling coefficient of the device. Basically, four different electrode/layer combinations are possible as shown in Figure 4.
20 AlN Thin Film Electroacoustic Devices 19 IDTF FIDT IDTM MIDT a) b) c) d) Figure 4 Different IDT/Thin Film configurations. They are explained as follows: Case 1: IDTF means that the IDT s are located on top of the piezoelectric film without a short circuiting plane Case 2: FIDT means that the IDT s are located under the piezoelectric film without a short circuiting plane Case 3: IDTM means that the IDT s are located on top of the piezoelectric film with a short circuiting plane under the latter Case 4: MIDT means that the IDT s are located under the piezoelectric film with a short circuiting plane on top of the latter As discussed above (see Section 2.1, Eq. (3)), the following relations are well known for piezoelectric materials. 2 2 (33) 2 C o C s ( Vo ) ( Vs ) Vo Vs K = = = 2 2 C o ( V ) Vo where Co and Cs are stiffness constants and Vo and Vs are the phase velocity of SAW at the electrically open surface (stiffened) and shorted surface (unstiffened), respectively. This approximation is useful to determine the coupling coefficient for SAW. Since Vo and Vs are obtained by the Campbell & Jones method discussed above, K² is easily calculated. For example, K² of the structure in Figure 4(a) is obtained from the SAW velocity, Vo, calculated by the free surface condition in Figure 4(a), and from the SAW velocity, Vs, calculated for the metallized region shorcircuiting the A1N surface as shown in Figure 4(d). o
SYNTHESIS AND PROPERTIES OF NEW SEMICONDUCTOR ALLOYS FOR LONG WAVELENGTH COHERENT EMITTERS ON GALLIUM ARSENIDE
UNIVERSITÀ DEGLI STUDI DI TRIESTE XVI CICLO DEL DOTTORATO DI RICERCA IN FISICA SYNTHESIS AND PROPERTIES OF NEW SEMICONDUCTOR ALLOYS FOR LONG WAVELENGTH COHERENT EMITTERS ON GALLIUM ARSENIDE DOTTORANDO
More informationUniversità degli Studi di Torino Scuola di Dottorato in Scienza ed Alta Tecnologia
Università degli Studi di Torino Scuola di Dottorato in Scienza ed Alta Tecnologia Development of a gaseous photon detector for Cherenkov imaging applications Elena Rocco ii 1 Università degli Studi di
More informationProperties of Electrons, their Interactions with Matter and Applications in Electron Microscopy
Properties of Electrons, their Interactions with Matter and Applications in Electron Microscopy By Frank Krumeich Laboratory of Inorganic Chemistry, ETH Zurich, VladimirPrelogWeg 1, 8093 Zurich, Switzerland
More informationDynamics and synchronization of two and three delaycoupled semiconductor lasers
Dynamics and synchronization of two and three delaycoupled semiconductor lasers Tesis presentada por M. en C. Diana Alejandra Arroyo Almanza Asesor Alexander. Pisarchik Como requisito para obtener el
More informationPRINTED CIRCUIT BOARD DESIGN
CHAPTER 6 PRINTED CIRCUIT BOARD DESIGN 6.1 INTRODUCTION The designers are key personnel in the development of a new electronic product but they are not the only ones. A successful product depends on an
More informationSingleElectron Devices and Their Applications
SingleElectron Devices and Their Applications KONSTANTIN K. LIKHAREV, MEMBER, IEEE Invited Paper The goal of this paper is to review in brief the basic physics of singleelectron devices, as well as their
More informationQuantum Point Contacts
SEMICONDUCTORS AND SEMIMETALS VOL 35 CHAPTER 2 Quantum Point Contacts H. van Hauten and C. W. J. Beenakker PHILIPS RESEARCH LABORATORIES EINDHOVEN THE NETHERL \NDS B J. van Wees DEPARTMENT OE APPLIED PHYSICS
More informationMagnetron Theory of Operation
Magnetron Theory of Operation Theory of Operation A magnetron is a high power microwave oscillator in which the potential energy of an electron cloud near the cathode is converted into r.f. energy in a
More informationBreakdown of Local Thermodynamic Equilibrium...
II Stellar Atmospheres Copyright (2003) George W. Collins, II 15 Breakdown of Local Thermodynamic Equilibrium... Thus far we have made considerable use of the concepts of equilibrium. In the stellar interior,
More informationAn introduction to quadrupole timeofflight mass spectrometry
JOURNAL OF MASS SPECTROMETRY J. Mass Spectrom. 21; 36: 849 865 SPECIAL FEATURE: TUTORIAL An introduction to quadrupole timeofflight mass spectrometry Igor V. Chernushevich, Alexander V. Loboda and Bruce
More informationField Estimation of Soil Water Content
Field Estimation of Soil Water Content A Practical Guide to Methods, Instrumentation and Sensor Technology VIENNA, 2008 TRAINING COURSE SERIES30 TRAINING COURSE SERIES No. 30 Field Estimation of Soil Water
More informationThe Prospects of Alternatives to Vapor Compression Technology for Space Cooling and Food Refrigeration Applications
PNNL19259 Prepared for the U.S. Department of Energy under Contract DEAC0576RL01830 The Prospects of Alternatives to Vapor Compression Technology for Space Cooling and Food Refrigeration Applications
More informationCHAPTER 12: PRINTED CIRCUIT BOARD (PCB) DESIGN ISSUES
PRINTER CIRCUIT BOARD ISSUES CHAPTER 12: PRINTED CIRCUIT BOARD (PCB) DESIGN ISSUES INTRODUCTION 12.1 SECTION 12.1: PARTITIONING 12.3 SECTION 12.2: TRACES 12.5 RESISTANCE OF CONDUCTORS 12.5 VOLTAGE DROP
More informationTimeCorrelated Single Photon Counting
Technical Note TimeCorrelated Single Photon Counting Michael Wahl PicoQuant GmbH, Rudower Chaussee 29, 12489 Berlin, Germany, info@picoquant.com The Principle of TimeCorrelated Single Photon Counting
More informationHighSpeed Digital System Design A Handbook of Interconnect Theory and Design Practices
HighSpeed Digital System Design A Handbook of Interconnect Theory and Design Practices Stephen H. Hall Garrett W. Hall James A. McCall A WileyInterscience Publication JOHN WILEY & SONS, INC. New York
More informationNonVolatile Memory Based on Solid Electrolytes
NonVolatile Memory Based on Solid Electrolytes Michael N. Kozicki, Chakravarthy Gopalan, Murali Balakrishnan, Mira Park, and Maria Mitkova Center for Solid State Electronics Research Arizona State University
More informationHALL EFFECT SENSING AND APPLICATION
HALL EFFECT SENSING AND APPLICATION MICRO SWITCH Sensing and Control 7DEOHRI&RQWHQWV Chapter 1 Hall Effect Sensing Introduction... 1 Hall Effect Sensors... 1 Why use the Hall Effect... 2 Using this Manual...
More informationHigh Strain R. 33. High Strain Rate and Impact Experiments. Part D 33
1 High Strain R 33. High Strain Rate and Impact Experiments Part D 33 K. T. Ramesh Experimental techniques for highstrainrate measurements and for the study of impactrelated problems are described. An
More informationDisposable Smart Lab on a Chip for PointofCare Clinical Diagnostics
Disposable Smart Lab on a Chip for PointofCare Clinical Diagnostics CHONG H. AHN, JINWOO CHOI, GREGORY BEAUCAGE, JOSEPH H. NEVIN, MEMBER, IEEE, JEONGBONG LEE, ANIRUDDHA PUNTAMBEKAR, AND JAE Y. LEE
More informationAN0971 APPLICATION NOTE
APPLICATION NOTE One Technology Way P.O. Box 9106 Norwood, MA 020629106, U.S.A. Tel: 781.329.4700 Fax: 781.461.3113 www.analog.com Recommendations for Control of Radiated Emissions with isopower Devices
More informationAgilent Network Analyzer Basics
Agilent Network Analyzer Basics 2 Abstract This presentation covers the principles of measuring highfrequency electrical networks with network analyzers. You will learn what kinds of measurements are
More informationWMR Control Via Dynamic Feedback Linearization: Design, Implementation, and Experimental Validation
IEEE TRANSACTIONS ON CONTROL SYSTEMS TECHNOLOGY, VOL. 10, NO. 6, NOVEMBER 2002 835 WMR Control Via Dynamic Feedback Linearization: Design, Implementation, and Experimental Validation Giuseppe Oriolo, Member,
More informationSensing and Control. A Process Control Primer
Sensing and Control A Process Control Primer Copyright, Notices, and Trademarks Printed in U.S.A. Copyright 2000 by Honeywell Revision 1 July 2000 While this information is presented in good faith and
More informationPatterning: Principles and Some New Developments**
Patterning: Principles and Some New Developments** By Matthias Geissler and Younan Xia* This article provides an overview of various patterning methodologies, and it is organized into three major sections:
More informationElectrowetting: from basics to applications
INSTITUTE OF PHYSICSPUBLISHING J.Phys.: Condens. Matter 17 (2005) R705 R774 JOURNAL OFPHYSICS: CONDENSED MATTER doi:10.1088/09538984/17/28/r01 TOPICAL REVIEW Electrowetting: from basics to applications
More informationSYLLABUS. Cambridge International AS and A Level Physics. Cambridge Advanced
SYLLABUS Cambridge International AS and A Level Physics 9702 For examination in June and November 2015 Cambridge Advanced Changes to syllabus for 2015 This syllabus has been updated. Significant changes
More informationIrreversibility and Heat Generation in the Computing Process
R. Landauer Irreversibility and Heat Generation in the Computing Process Abstract: It is argued that computing machines inevitably involve devices which perform logical functions that do not have a singlevalued
More informationUnderstanding the FiniteDifference TimeDomain Method. John B. Schneider
Understanding the FiniteDifference TimeDomain Method John B. Schneider June, 015 ii Contents 1 Numeric Artifacts 7 1.1 Introduction...................................... 7 1. Finite Precision....................................
More informationAcoustic Doppler Current Profiler Principles of Operation A Practical Primer
Acoustic Doppler Current Profiler Principles of Operation A Practical Primer P/N 951606900 (January 2011) 2011, Inc. All rights reserved. Revision History: January 2011 Corrected Equation 9, page 34.
More informationMobile telecommunication base stations exposure to electromagnetic fields
COST 244bis Short Term Mission on Base Station Exposure Page 1 Dedicated to Ulf Bergqvist Mobile telecommunication base stations exposure to electromagnetic fields Report of a Short Term Mission within
More information